This is an accelerated laboratory corrosion test method that can be used to determine the corrosion resistance of automotive assemblies and components. It is cyclic in nature, i.e.; test specimens are exposed to changing climates over time.
Test specimens are placed in an enclosed chamber and exposed to a changing climate that comprises of a relatively short period of salt spray, followed by exposure to hot/humid and hot/dry atmospheres. The entire test cycle comprises of a main cycle and a sub-cycle. 1 entire test cycle takes 24 hours to execute. The number of entire cycle repeats and therefore the test duration is variable.
The main test cycle begins with 10 minutes exposure to a continuous indirect spray of salt water solution, in a chamber temperature of +35C . This is followed by 155 minutes of air drying at +60C. This is followed by 75 minutes exposure to a high humidity climate of 95%RH at +60C.
This is then followed by a repetitive sub-cycle comprising of 160 minutes of exposure to an air drying at +60C, followed by 80 minutes exposure to a humid climate of 95%RH at +60C. This sub-cycle is repeated 5 times in total, before the main test cycle starts again.
Necessary cookies are absolutely essential for the website to function properly. This category only includes cookies that ensures basic functionalities and security features of the website. These cookies do not store any personal information.
Any cookies that may not be particularly necessary for the website to function and is used specifically to collect user personal data via analytics, ads, other embedded contents are termed as non-necessary cookies. It is mandatory to procure user consent prior to running these cookies on your website.